Transcript of "Cements and adhesives for all ceramic restorations"
C e m e n t s an d A d h e s i v e sf o r Al l - C e r a m i cRestorationsAdriana P. Manso, DDS, MSc, PhDa,b,Nelson R.F.A. Silva, DDS, MSc, PhDc,Estevam A. Bonfante, DDS, MSc, PhDd, Thiago A. Pegoraro, DDS, PhDe,Renata A. Dias, DDSc, Ricardo M. Carvalho, DDS, PhDf,* KEYWORDS Dental cements Esthetic dentistry Resin-based cements Simplified adhesives systems Incompatibility Ceramics SilanationDental luting cements are designed to retain restorations, appliances, and post andcores in a stable and, presumably, long-lasting position in the oral environment.Retention mechanisms are reported to be chemical, mechanical (friction), and micro-mechanical (hybridized tissue), but they are usually a combination of two or threemechanisms, depending on the nature of the cement and of the substrate. Amongdental luting cements commercially available, there are resin-based and nonresin-based cements. They must have for their acceptable clinical performance adequateresistance to dissolution, strong bond through mechanical interlocking and adhesion,high strength under tension, good manipulation properties, and also be biologicallycompatible with the substrate.1,2 Traditionally, zinc phosphate cement has been regarded as the most popular mate-rial, despite its disadvantages as low hardness, solubility and lack of adhesion.3 This work was partially supported by Cap grants # 300305/0-4, Brazil, and FAPESP # 04/1263-0, and # 2010/06152-9 Brazil. a Department of Operative Dentistry, University of Florida, College of Dentistry, 1600 Archer Road, Gainesville, FL 32610, USA b ´ ˜ Instituto HNary, Al. Octavio Pinheiro Brisola, 12-67, 17012-901, Bauru, Sao Paulo, Brazil c Department of Prosthodontics, New York University College of Dentistry, 345 East 24th Street, New York, NY 10010, USA d Department of Prosthodontics, UNIGRANRIO University, School of Dentistry, Rio de Janeiro, Brazil e ˆ Department of Prosthodontics, University Center, CESMAC, Rua Conego Machado, 918, Farol, Maceio, Alagoas, 57051160, Brazil f ˜ ´ Department of Prosthodontics, University of Sao Paulo, Bauru School of Dentistry, Al. Otavio ˜ P. Brisola 9-75, Bauru, Sao Paulo 17012901, Brazil ´ ´ ˜ * Corresponding author. Departamento de Protese, Al. Otavio P. Brisola 9-75, Bauru, Sao Paulo 17012901, Brazil. E-mail address: email@example.com Dent Clin N Am 55 (2011) 311–332 doi:10.1016/j.cden.2011.01.011 dental.theclinics.com 0011-8532/11/$ – see front matter Ó 2011 Elsevier Inc. All rights reserved.
312 Manso et al Although the final marginal accuracy of all-ceramic systems processes (computer-aided design [CAD]/computer-aided manufacturing [CAM] especially) have significantly improved, these still result in larger internal gaps than cast crowns, possibly resulting in thicker cement layers4 and poorer frictional retention to the abutments. These would be critical challenges for zinc phosphate cement because of its solubility and lack of adhesiveness. Although zinc–phosphate has been indicated for some all-ceramic systems (ca In-Ceram [VITA Zahnfabrik H. Rauter GmbH Co KG, Bad Sackingen, ¨ Germany], Procera [Nobel Biocare, Switzerland], Cercon [DeguDent, Hanau, Germany], Lava [3M ESPE, St Paul, MN, USA]), long-term clinical data are yet to be published. Glass ionomer cements are also of great interest for clinicians. These cements exhibit several clinical advantages,5 including physicochemical bonding to tooth structures,5,6 long-term fluoride release, and low coefficients of thermal expansion.5,7 However, their low mechanical strength compromises their use in high-stress-bearing areas.5,8 Glass ionomer cements can be used to cement core-reinforced ceramics such as those also allowed to be cemented with zinc phosphate. However, glass ion- omer cements would not suit well for ceramics requiring support from the cement. Therefore resin-based cements have become popular, because they have the poten- tial to address the disadvantages of solubility, support, and lack of adhesion described for previous materials.1 Restorative dentistry constantly undergoes changes, and no currently available cement is ideal for all situations. The advent of adhesive luting cements has consider- ably expanded the scope of fixed prosthodontics. This article will focus on resin- based cements as luting agent for all-ceramic systems, due to the important role the cement plays in the final clinical success of such treatment modality. RESIN CEMENTS AND ADHESIVE INTERFACES Resin cements have become popular clinically because of their ability to bond both the tooth structure and restoration. Bonded indirect restorations constitute a substantial part of contemporary dentistry.9 The successful use of resin cements depends on several aspects related to the bonding mechanisms to both dental tissues and resto- rations. The scientific knowledge of the materials currently available as well as the acknowledgment of their limitations and indications are key factors for durable resto- rations. Several new luting cements and ceramic systems have been introduced in the last few years, and their chemistry and structural characteristics are fundamental to produce an optimal and reliable bonding to both tooth and restoration interfaces. Resin Cements: Chemistry and Properties Table 1 summarizes various resin-based cements with their respective characteristics and chemical compositions. Resin-based luting cements were primarily based on acrylic resin chemistry. Their subsequent development, however, has been based on the chemistry of resin composites and adhesives.10 Currently, several new resin cements are available in the market. These are offered in a wide variety of bonding mechanisms, curing modes, indications, and features (see Table 1). The choice of a particular resin cement requires understanding of the material’s characteristics as well as how it performs individually and integrated in the restorative system. There are two main categories of resin luting cements: the conventional resin luting cements, which have no inherent adhesion to tooth structure and require a bonding agent, and the self-adhesive resin cements, which do not require a separate bonding treatment to the dental substrate.
Cements and Adhesives 313Conventional resin luting cementsSince the 1970s, resin cements have been formulated based on dimethacrylate resinchemistry as two-paste systems, which are easy to mix and cure at roomtemperature.3 Their bonding to tooth structure relies on the use of etch-and-rinse orself-etch adhesives. Composition is usually a mixture of dimethacrylate monomers,inorganic fillers (60% to 70% by weight), and initiator. Silica or high molecular weightoligomers may also be added to modify the rheological properties and achieveoptimum handling characteristics. Examples of their clinical applications includemetal-based crowns and bridges, zirconia and alumina framed crowns, fiber posts,and cast metal post and core. Because of the importance of light- and dual-curingsystems, a separate topic was created to address their clinical application and poly-merization mechanisms.Curing protocols and its clinical relevance Light-cured Conventional resin cements can be exclusively light-cured. Whencomparing cements, light-cure products offer the clinical advantages of extendedworking time, setting on demand, and improved color stability. However, the use oflight-cure only cements is limited to situations such as cementing veneers or shallowinlays, where the thickness and color of the restoration do not affect the ability of thecuring light to polymerize the cement.11,12 Dual-cured Dual-cured resin cements are often provided in two-paste systems (seeTable 1). Dual-cure resin cements are indicated when delivering restorations wherematerial characteristics may inhibit sufficient light energy from being transmitted tothe cement.13 In these situations, light intensity reaching the cement may be sufficientto trigger the light-activated polymerization process, but a self-polymerized catalyst isneeded to ensure maximal cure. The delivery method usually involves mixing of pasteto paste (see Table 1). One of the pastes contains a reducing amine and a photo initi-ator. The other paste contains peroxide, usually benzoyl peroxide. In an interestingvariation of the initiator system, the anaerobic cements begin polymerization onlywhen the ambient oxygen supply is cut off after placement of the prosthetic device.This feature provides extended working and setting times and offers easy removalof excess materials.14,15 Although the dual-curing concept seems to be attractive,several issues have been brought up in the dental literature regarding its performance,and these concerns are going to be addressed throughout the text. Little has been published on the light-curing potential of dual-cure cements. Whileearlier research suggests that auto-cure alone is not sufficient to achieve maximumcement hardening,16,17 recent literature indicates that the curing kinetics of dual-cure resin cements is more complex than previously thought.18 Studies indicate thatlight-activating some dual-cure cements appears to interfere with the self-cure mech-anism and restrict the cement from achieving its maximum mechanical properties.19,20 Some dual-cure cements show their self-curing mechanism to be somehow limitedwhen immediately light-activated in the dual-cure mode. This limitation may compro-mise the final mechanical properties of the resin cements.19 This information is of greatimportance for the clinical practice, since light activation is always recommended bythe manufacturer. It remains to be demonstrated whether the same phenomenonoccurs with all resin-based cement systems. While such information is not available,it is advisable to delay the light-curing procedure of dual-cure cements to themaximum time clinically possible.20 In this way, self-curing progress will be furtheralong, to a point when light activation no longer interferes with the self-curing kinetics.The ideal time frame between mixing and the light-activation has not yet been deter-mined, but some studies have shown that light-curing 5 to 10 minutes after mixing
314 Manso et alTable 1Representative resin cement systemsProducts Company Adhesive Delivery Curing CompositionBistite II DC Tokuyama Primer 1A1 Paste/paste Dual Silica-zirconia (77% weight) filler, (Tokyo, Japan) 1B/primer 2 dimethacrylate, MAC-10 (adhesive promoter), initiatorCalibra Dentsply/Caulk Prime and Paste/paste Dual Base: barium boron fluoralumino silicate (Milford, DE, USA) bond NT glass, bis-phenol A diglycidylmethacrylate, polymerizable dimethacrylate resin, hydrophobic amorphopus silica, titanium dioxide, di-camphoroquinon Catalyst: barium boron fluoralumino silicate glass, bis-phenol A diglycidylmethacrylate, polymerizable dimethacrylate resin, hydrophobic amorphopus silica, titanium dioxide, benzoyl peroxideCB Cement Bisco All-bond 2 Paste/paste Self Base: Bis-GMA, ethoxylated bis-gma, (Schaumburg, IL, USA) one step dual syringe trietheleneglycol dimethacrylate, fused silica, glass filler, sodium fluoride Catalyst: Bis-GMA, trietheleneglycol dimethacrylate, fused silicaChoice 2 Bisco All-bond/one Paste Light Strontium glass, amorphous silica, step Bis-GMADuo-Link Bisco All-bond 2 Paste/paste dual Dual Base: Bis-GMA, triethyleneglycol one step/plus syringe; automix dimethacrylate, urethane dimethacrylate, glass filler Catalyst: Bis-GMA, triethyleneglycol dimethacrylate, glass fillerBisCem Bisco Self-adhesive Paste/paste dual Dual Bis (hydroxyethyl methacrylate) syringe; automix phosphate (base), tetraethylene glycol dimethacrylate, dental glass
NX 3 Nexus Kerr (Washington, DC, USA) Optibond solo Paste/paste dual Dual Uncured methacrylate ester monomers, plus optibond syringe; automix nonhazardous inert mineral fillers, all-in-one nonhazardous activators and stabilizers, and radiopaque agentMaxcem Kerr Self-adhesive Paste/paste dual Dual GPDM (glycerol dimethacrylate syringe; automix dihydrogen phosphate), comonomers (mono-, di-, and tri-functional methacrylate monomers), stabilizer, barium glass fillers, fluoroaluminosilicate glass filler, fumed silica (filer load 67% weight, particle size 3.6 mmSuper Bond CB Sun Medical Monomer/catalyst 4 drops of monomer/1 Self MMA (methyl methacrylate), (Grand Prairie, TX, USA) V/polymer drop of catalyst 4-methacryloxyethyl trimellitate powder s/1 small cup of anhydride (4-META), tri-nbutylborane standard measuring (TBB- catalyst) spoonClearfil Esthetic Kuraray Self-etch DC bond Paste/paste dual Dual Paste A: bis-phenol A Cement (Tokyo, Japan) system syringe; automix diglycidylmethacrylate, TEGMA, methacrylate monomers, silanated glass filler, colloidal silica Paste B: bis-phenol A diglycidylmethacrylate, TEGMA, methacrylate monomers, silanated glass filler, silanated silica, colloidal silica, benzoyl peroxide, CQ, pigments Cements and Adhesives (continued on next page) 315
316 Manso et alTable 1(continued )Products Company Adhesive Delivery Curing CompositionPanavia F 2.0 Kuraray ED primer Paste/paste Dual Paste A: 10-methacryloyloxydecyl, dihydrogen phosphate, hydrophobic aromatic dimethacrylate, hydrophobic aliphatic dimethacrylate, hydrophilic aliphatic dimethacrylate, silanated silica filler, silanated colloidal silica, dl- camphorquinone, catalysts, initiators Paste B: hydrophobic aromatic dimethacrylate, hydrophobic aliphatic, dimethacrylate, hydrophilic aliphatic dimethacrylate, silanated barium glass filler, catalysts, accelerators, pigmentsBreeze Pentron Self-adhesive Paste/paste dual Dual Mixture of bis-GMA, UDMA, TEG-DMA, Clinical Tech (Orange, CA, USA) syringe; automix HEMA, and 4-MET resins, silane-treated bariumborosilicate glasses, silica initiators, stabilizers and UV absorber, organic and/or inorganic pigments, opacifiersGCem GC Self-adhesive Capsules Dual Powder: fluoroaminosilicate glass, (Tokyo, Japan) initiator, pigment Liquid: 4-MET, phosphoric acid ester monomer, water, UDMA, dimethacrylate, silica powder, initiator, stabilizerEmbrace Pulpdent Self-adhesive Standard syringe Dual Uncured acrylate resins, amorphous silica, WetBond (Watertown, MA, USA) or automix sodium flurideMonoCem Shofu Dental Self-adhesive Paste/paste dual Dual Not available (San Marcos, CA, USA) syringe; automix
Multilink Sprint Ivolcar/Vivadent (Schaan, Principality of Self-adhesive Paste/paste dual Dual Dimethacrylates and acidic monomers, Liechtenstein) syringe; automix barium glass, ytterbium trifluoride, silicon dioxide, mean particle size is 5 mm, total volume of inorganic fillers is w48%Multilink Ivoclar/Vivadent Primer A 1 B Paste/paste dual Self Dimethacrylate and HEMA, barium glass syringe; automix filler, silicon dioxide filler, ytterbium trifluoride, catalysts and stabilizers, pigmentsVariolink II Ivoclar/Vivadent Excite adhesive Paste/paste Dual Paste of dimethacrylates, inorganic fillers, ytterbiumtrifluoride, initiators, stabilizers and pigments; (Bis-GMA, triethylene glycoldimethacrylate, urethanedimethacrylate, benzoyl peroxide)Rely X ARC 3M ESPE (St Paul, MN, USA) Adper single Paste/paste; Dual Bisphenol-A-diglycidylether bond clicker dimethacrylate (BisGMA), triethylene glycol dimethacrylate (TEGDMA), polymer, zirconia/silica filler, filler loading approximately 67.5% by weight, particle size for the filler is 1.5mm.Rely X Unicem 3M ESPE Self-adhesive Capsules (Aplicap: Dual Powder: glass fillers, silica, calcium 0.01 mL; Maxicap: hydroxide, self-curing initiators, 0.36 mL) pigments, light-curing initiators (filler Cements and Adhesives load 72% weight, particle size 9.5 mm); Liquid: methacrylated phosphoric esters, dimethacrylates, acetate, stabilizers, self-curing initiatorsRely X Unicem 3M ESPE Self-adhesive Paste/paste; Clicker Dual Glass powder, methacrylated phosphoric acid esters, triethylene glycol dimethacrylate (TEG-DMA), silane treated silica, sodium persulfate 317
318 Manso et al does not seem to interfere with final cure and properties, at least for most of the cements evaluated.19 It is interesting to note that there is no direct correlation between alterations in the degree of conversion (DC) caused by different curing modes and changes in the mechanical properties of the resin cements.19 The lack of linear correlation between DC, properties, and density of crosslink in the polymer has also been reported elsewhere.21 However, cements that do not cure properly with light activation or have a compromised self-cure reaction may experience adverse chemical reactions and permeability issues when associated with simplified adhesive systems.20 This clinically implies that the longer the resin cement takes to set, the greater will be the chance of adverse effects when coupling resin cements to simplified adhesives. To overcome these problems, clinicians have been advised to use three-step etch and rinse or two-step self-etch adhesives.20,22–24 When using these systems, adverse chemical reaction and permeability are prevented by the nonacidic and relatively higher hydrophobic characteristics of the bonding resin that comprise the last step of the application of such systems.22 Clinical trials are necessary to demonstrate how these issues may affect the long-term performance of different combinations of adhesives and cements. Concerns on mixing and working time of dual-cure cements Resin-based cements are formulated to provide the handling characteristics required for particular applica- tions. The setting mechanism of dual-cure resin cements is usually based on redox reaction of benzoyl peroxide with aromatic tertiary amines (represented by catalyst and base paste, respectively). At least one paste contains the light-sensitive compound (camphorquinone [CQ]) responsible for initiating the light-cure setting mechanism. After the pastes are mixed together, and until light is provided, the working time is controlled by the ratio between inhibitors of the self-curing reaction and the amount of peroxide and aromatic tertiary amines. Both inhibitors and perox- ides are organic chemical compounds susceptible to degradation upon storage. Therefore, dual-cure resin cements have a limited shelf-life and the setting mechanism of those cements may fluctuate during that time, depending on the conditions of storage that might alter the reactive potential of such components. In vitro evidences indicate that both working time (WT) and setting time (ST) may be significantly altered upon storage,19 particularly if the storage temperature is far above the recommended ( 18 –22 C). In one study, some cements presented shortened WT/ST, while others presented extended WT/ST after the kits were purposely aged for 12 weeks at 37 C.19 This occurred because of the instability of the components during storage. Degrada- tion of peroxide would extend the WT/ST, and degradation of inhibitors would shorten them. The implications of such changes on the mechanical properties of the resin cements are yet unclear. However, clinicians handling resin cements with shortened WT may experience some clinical difficulties when luting multiple crowns, for example. Conversely, increased adverse chemical reaction and permeability problems may be expected for resin cements with extended WT and ST used in combination with an acidic and permeable simplified adhesive system. This is mostly because the extended ST allows the uncured cement longer time in contact with the acidic adhe- sive, thus prolonging the adverse reaction. Bonding mechanisms and incompatibility issues of dual-cure cements Most adhesive systems used with resin-based cements are simplified adhesive systems, because of clinical trends for reduced steps during adhesive procedures. These simplified adhe- sives are basically of two types: the etch-and-rinse, single-bottle systems and the all- in-one self-etch adhesives. They are both somewhat acidic and hydrophilic in nature.
Cements and Adhesives 319During cementation, the acidic groups in the uncured layer of simplified adhesiveagents (due to presence of oxygen) compete with peroxides for aromatic tertiaryamines of the luting agent, resulting in an acid–base reaction between the adhesiveand the resin cement. This reaction minimizes proper copolymerization between thetwo, and the longer the cement takes to cure, the more extent is the compromisingeffect.25–27 Additionally, the hydrophilic characteristics of such adhesive systemsfunction as permeable membranes. This hydrophilic behavior permits the flux of waterthrough the adhesive after polymerization.28,29 The presence of water at the interfacebetween the adhesive and the cement compromises the total bonded area and properpolymerization of the cement. Water droplets may accumulate at the interface andthen function as stress raisers, leading to failure of the adhesive–cement interface(Fig. 1).28 This permeability problem could be partially solved by the application ofan intermediate layer of a relatively more hydrophobic, nonacidic low viscosity resinseparating the acidic layer of adhesive from the composite resin cement.28,30 Thewater that accumulates at the interface derives from the hydrated dentin underneath.The negative effect of such water permeation on the bond strength of resin cements todentin could be confirmed in in vitro studies.28,29 Those studies demonstratedimproved bond strengths when the teeth were purposely dehydrated in ascendingethanol series before bonded. As such dehydration of dentin is impossible to achievein daily practice, clinicians are advised to use less permeable adhesive systems suchas three-step etch and rinse or two-step self-etch when bonding self- or dual-curedresin cements to dentin.28,30 The major advantage of these systems is that they includea layer of a relatively more hydrophobic and nonacidic resin as the third or second step.This additional layer will not cause adverse reaction with the basic amines of the cementand will reduce the permeability of the adhesive layer.31,32 The incompatibility issue hasbrought up concerns for several clinical procedures. The worst clinical scenario wouldoccur when luting posts using simplified adhesives associated with dual-cured resincements (see Fig. 1). Proper bonding to the apical portion might be severely compro-mised by the adverse interactions between adhesive and luting composite due to a lackof light exposure. Without light activation, dual-cure resin cements will actually functionas exclusively self-cure cements. In this mode, the cement will take longer to cure, andthis allows more time for the adverse reaction and transudation of water from dentin tooccur. A similar situation occurs when the cement takes longer to set because of alter-ations in the WT/ST caused by inadequate storage conditions, as described previously.Based on those limitations, some studies have suggested the development of a specificbonding system for this purpose.31,32 Recent studies have shown that the push-outresistance of posts luted with resin cements was similar, regardless of the use of adhe-sive systems to bond to root dentin.31,32 A more predictable, truly adhesive lutingprocedure can only be achieved when clinicians combine the use of resin cementswith three-step etch and rinse or two-step self-etch bonding systems. Self-adhesiveresin cements have been strongly recommended to lute posts and crowns as an alter-native to conventional luting systems, avoiding incompatibility and permeability issuesdue to wrong combinations of adhesives and cements. When cementing inlays, onlays, and crowns, immediate dentin sealing concept33may be a useful clinical alternative to overcome the incompatibility and permeabilityissues. Further details on this approach can be found elsewhere.20,34,35Self-adhesive resin cementsThe simplification to only one step of resin luting procedures was achieved with theself-adhesive resin cements.36 This system uses a dual-cure concept for polymeriza-tion, and no pretreatments using bonding agents on the tooth surface is required,
320 Manso et al Fig. 1. This sequence of micrographs shows the in vivo morphologic characteristics of root dentin during postcementation procedures using an etch-and-rinse two-step adhesive system. Observations were made in (A) cervical, middle, and apical thirds (dotted circles) of the root canal by means of an impression with a polyvinyl siloxane material taken imme- diately after (B) postspace preparation, (C) etching with phosphoric acid, and (D) application of the adhesive system. The impression of the root canal was then positioned in a container allowing an epoxy resin to be poured covering up to half of the impression. After gold sput- tering, the samples were taken to a scanning electron microscope at 1000 Â magnification for evaluation. After postspace preparation, the anticipated presence of a smear layer (arrows) was observed in the (Bc) cervical and (Bm) middle thirds, but noticeably higher amounts were detected at the apical section (Ba). Remarkably, etching with phosphoric acid did not effectively remove the smear layer at either cervical, middle, or apical thirds (Cc, Cm, Ca, respectively), and dentinal tubules do not seem to be available for hybridiza- tion. Micrographs taken after subsequent layering of an adhesive system with a microbrush revealed evidence of water permeation and blistering (pointers) protruding from the dentin surface, and they were more frequently observed in (Dc) cervical and (Dm) middle thirds relative to the (Da) apical third. One possible reason may be the progressively lower number and diameter of dentinal tubules toward the apical area and the reduced permeability in this area. making its application clinically attractive. Self-adhesive resin cements are claimed to be moisture-tolerant, to release fluoride, and to present no postoperative sensitivity.37 Thus, all these factors combined fit to the clinical demand for simplification and less technique sensitiveness.38
Cements and Adhesives 321 The first of this class of materials was introduced as a powder–liquid materialprovided in unit–dose capsule that had to be triturated (RelyX Unicem [3M ESPE, StPaul, MN, USA]), and newer paste-paste versions have been commercialized (seeTable 1). The setting reaction is initiated by light exposure and by the self-curingmechanism. In general, the initial low pH is neutralized through reactions betweenacid groups and alkaline filler and tooth apatite. Lower bond strengths to enamelcompared with dentin have been reported, and this fact may limit the use of self-adhesive resin cements for bonding veneers.15,38 Moreover, esthetic veneers andminimally invasive restorations require longer working time for positioning anddemand more esthetic and shade availability than the ones that have been providedfor self-adhesive kits.Bonding mechanism of self-adhesive cements Conventional resin cements require anadhesive agent to mediate bonding to tooth structure, which can be either etch-and-rinse (three- or two-step) or self-etch adhesive system (two- or one-step). It seems thatthe more steps involved in the bonding procedure for both bonding approaches, themore stable is the bonded interface produced.39 Conversely, when more clinical stepsare required, it is also more critical to keep the bonding substrates properly isolated;additionally the chances are higher for technique sensitivity. Self-adhesive resin cements do not require the bonding step. The acidity of thecement is strong enough to promote hybridization with the tooth structure. While stillfluid, the acidic groups of the monomer dissolve the smear layer, which allows pene-tration of the cement into the dentinal tubules, thus providing a good hybrid layer andgood adhesion. Micromechanical retention and chemical interaction between acidicgroups and hydroxy-apatite are expected. It has been reported that self-adhesivecement showed chemical interaction with Ca ions derived from hydroxy-apatite.40Enamel bonding with a self-adhesive cement produced lower bond strengths thanconventional resin cements but higher than glass–ionomer. It may be considered asan alternative to glass–ionomer luting cement for cementation of high-strengthceramic or metal-based restorations, but it might not be ideal for luting restorationssuch as veneers, inlays, and partial crowns if a considerable enamel surface area ispresent.41 The use of phosphoric acid for etching enamel before the application ofself-adhesive resin cement can result in bond strengths comparable to conventionalresin cements.42 However, previous etching can be detrimental for bond strengthsto dentin.43 Although self-adhesive and conventional resin cement–dentin interfacesare morphologically different,43,44 self-adhesive cements have been reportedto perform equally effective when compared with most conventional resincements.38,45,46 There is still a need for a more long-term clinical evaluation of self-adhesive cements.Resin Cement and Water Sorption PhenomenonWhen an all-ceramic crown is cemented, the assembly ceramic/cement/adhesive/tooth will be subjected to a watery environment. Resin cements should not onlyhave low solubility, but also low water sorption because of esthetic and functionalreasons.47 The water sorption phenomenon has been demonstrated to have an impor-tant effect on the properties of resin cements after long periods of time.48,49 Watersorption diminishes significantly the flexural strength of resin composites. The reduc-tion of flexural strength as well as modulus of elasticity50 may be critical for thick areasof resin cement. Scientific evidences show that absorbed water works as a plasticizerfor the cements and, therefore, may create unsupported areas underneath restorationand consequently increase the chance of fracture of the restoration under mastication
322 Manso et al forces. Clinicians should keep as thin as possible the cement film to minimize the consequences of the plasticizing phenomenon for resin cements.51 The water sorption may also result in hygroscopic expansion50,52 of the cement, but the consequences of hygroscopic expansion on the long-term durability of dental cements, and conse- quently all-ceramic restoration, remain unknown. Clinicians should be aware that cements that present extended working time or setting time, do not cure properly with light activation, or have a compromised self- cure mechanism will more severely suffer with hygroscopic expansion issues. Incom- plete polymerization and nonconversion of monomer may result in loss of resin, and this may affect the biologic compatibility of the resin material.53 Scientific evidence54 has demonstrated that reducing the exposure time for polymerization of light-cure cements to 75% of that recommend by the manufacturer may facilitate fluid uptake and dissolution of the resin. Therefore, all measures should be taken to permit maximum polymerization of resin cements to minimize the water sorption phenom- enon and its consequences. Vrochari and collaborators55 have recently evaluated water sorption and solubility of several cements. The authors observed that materials with similar polymerization mechanisms may perform differently during their interaction with water. Thus, clini- cians are advised to be aware whether the resin-based cements to be chosen follow the International Organization for Standardization (ISO) standards regarding water sorption performance. Ideally, resin cements should present the lowest water sorption and solubility values possible. Film Thickness of Resin-Based Cements The importance of resin cement film thickness currently relies on the fact that most of the ceramic materials have considerable internal space. The effect of resin cement thickness on the fracture resistance of all-ceramic restorations is not completely established yet, but some studies have found some correlation between these factors. In 1994, Scherrer and colleagues56 reported that when resin cement thickness of 300 mm or more was present, a gradual decrease of the fracture strength was observed57 demonstrating that thick ceramic combined with minimal thickness of luting composite provided restorations with a favorable configuration with regard to prevent cracking.57 It was also demonstrated that glass–ceramics with thick cement layers exhibit significantly lower reliability after water aging.58 It seems that a thin cement thickness and proper bond to the ceramic structure is necessary for improved support and increased fracture resistance of all-ceramic crowns. Thicker cement layers have also been related to decreased bond strength of ceramic systems.59 Thus, clinicians are strongly advised to maintain a minimal film thickness (approximately 50 mm) to minimize the effects of water sorption and its consequences to the properties of the cement and respective support for the ceramic restoration. BONDING INTERFACE OF ALL-CERAMIC MATERIALS The development of new cement and adhesive techniques expanded the use of ceramics and indirect resin composites in dentistry. Bonding ceramic materials to enamel and dentin combined with the improved strength of these indirect restorative materials has produced restorations with improved mechanical integrity and reduced risk for fracture.60 Although a separate article of all-ceramic systems is included in this special issue for Dental Clinics of North America, a brief description of the ceramic materials characteristics will be presented to favor the understanding of their bonding strategies and mechanisms at the resin–cement/restorative material interface.
Cements and Adhesives 323Glass CeramicsFeldspathic glasses and Leucite-containing feldspathic glasses are still extensivelyused in veneers, inlays, and single anterior crowns. They offer excellent estheticoutcomes derived from their high translucency, fluorescence, and opalescence.However, these ceramics have drawbacks such as reduced strength and toughness.The glass–ceramic systems currently available are: Leucite-reinforced glass-ceramics (sintered, hot-pressed or CAD-CAM) with flex- ural strengths of up to 120 MPa, which is considered to be sufficient for veneers, anterior crowns and posterior inlays Fluormica glass-ceramics (CAD-CAM) with flexural strength of 120 to 150 MPa, which, combined with the adhesion to tooth tissues, may be adequate for selected posterior crowns. A significant improvement of the mechanical properties (flexural strength around350–450 MPa) of glass–ceramic systems was achieved with the development oflithium disilicate glass–ceramics (hot-pressed or CAD-CAM). Since the introductionof lithium disilicate ceramic to the market, the use of Leucite-reinforced glass–ceramics has declined. Moreover, besides the better mechanical properties andimproved esthetic outcomes, high bond strength can be achieved when bonded tothe tooth structure.60High-Strength Polycrystalline CeramicsAlthough high-strength polycrystalline ceramics (alumina and zirconia) broaden theapplications of all-ceramic systems to posterior crowns and bridges, randomized clin-ical trials and clinical experience have been controversial regarding long-termsurvival.61–67 As a result of its superior mechanical properties compared with alumina,zirconium became the first choice as a core or framework for all-ceramic restorations.However, it is imperative to mention that the bonding mechanisms to high-strengthceramics have been problematic as a result of lack of glass particles in its composi-tion. This issue and possible adhesion options to high-strength ceramics are dis-cussed in detail throughout the following section.Bonding strategies for all-ceramic systemsThe ability of a combination of resin cement/adhesive system to adhere to dentalceramics depends on the microstructure of the esthetic restoration and the surfacetreatment applied.68 While roughening the surface by grinding or airborne particleabrasion is considered a way for improved adhesion for most of the esthetic materials,silanation appears to be only effective for silica-based ceramics.69 A durable and reli-able bond for dental resin-bonded ceramics is usually attempted via two principalmechanisms: (1) micromechanical attachment to porosities originated from hydro-fluoric acid (HF) etching or (2) grit blasting, associated with a silane-coupling agent.Evaluations of bond strength between ceramic and resin composite have deriveddifferent conclusions about the effect of surface treatments. Controversy in theliterature70,71 relies on possible inefficacy or inactivity of the silane-coupling agentapplied and operator’s handling of the procedure. Meng and colleagues72 recentlydemonstrated that hydrofluoric acid treatment could enhance the bond durability ofresin/silanated glass ceramics, which might result from the increase of the chemicaladhesion area on the ceramic rough surface and subsequently reduced degradationspeed of the silane coupler, rather than the mechanical retention of the ceramic roughsurface.72
324 Manso et al Silane coupling Silane-coupling agents are bi-functional molecules capable of bonding to the hydroxyl groups on ceramic surfaces and copolymerizing with the organic portion of the resin cement or adhesive. Silane primers contain a silane agent (usually g-methacry- loxypropyl-trimethoxy silane), a weak acid, and high amounts of solvents. To be effec- tive, the silane agent must be hydrolyzed by the weak acid. Once hydrolyzed, silane primers have a limited shelf-life, and effectiveness progressively decays over time. The effectiveness of prehydrolyzed, single-bottle silane primers is, therefore, unpre- dictable if the user is not aware of when the solution was activated. Clinically, the only indicator seems to be the appearance of the liquid (ie, a clear solution is useful, while a milky-like solution should be discarded).69 However, alcoholic solution (one- bottle systems) stays transparent, and the signs of alterations cannot be identified. Therefore, two-bottle solutions are preferred. Practitioners should strictly respect expi- ration date and follow the manufacturers’ recommendations of silane systems. The understanding of how the silanation process occurs on ceramic surfaces is of great importance to improve effectiveness of silanes. When a silane is applied to a ceramic surface and dried, three different structures are formed at what is called interphase layer.73 The outermost layer consists of small oligomers that can be washed away by organic solvents or water at room temperature.71 Closer to the glass surface, there is another layer of oligomers that is hydrolysable. To avoid hydrolysis of this layer after cementation, which could compromise the coupling of the cement with the ceramic, some authors recommend it be removed with hot water before bonding to silanated ceramic.71,74 Attached to the glass there is a third layer, which is a mono- layer that is covalently bonded to the silica phase of the ceramic and is hydrolytically stable.70 This remaining monolayer of silane is not removed by these procedures, and it is responsible for the actual bond between the ceramic and the adhesive/cement system. Since it is not possible to clinically control the application of a monolayer of silane, undesirable excess must be removed before bonding. This can be achieved by several methods. One way is to apply the silane followed by hot air drying (50 C Æ 5 C) for 15 seconds for proper solvent evaporation. Then, rinse with hot water (80 C) for 15 seconds followed by another hot air drying for 15 seconds.74 This procedure would eliminate water and solvent and wash away any unreacted silane (excess) primer components.74 Alternatively, excess silane can be removed during the try-in step. The try-in procedure is known to be a contaminant step. Therefore, it has been rec- ommended to be done before silanation. Clinicians generally use the try-in step after receiving the surface-etched (hydrofluoric acid, HF) ceramic restoration from dental laboratories. However, the HF-treated ceramic surface is hydrophilic and more prone to be contaminated if the hydrophilic try-in paste is applied before the silanation step. Therefore, ceramic surfaces should be silanated before the try-in procedure. Once properly silanated, the ceramic surface becomes hydrophobic, and the try-in paste can be easily removed by ultrasonic cleansing. Current scientific evidences20 show that if the try-in step is done after silanation, bond strengths will increase significantly. This can be explained by the fact that the try-in procedure removes the excessive layers of silane from ceramic surface.20 The removal of excess permits proper coupling of the resin cement with the monolayer-silanated ceramic surface, thus improving the bond strength. Moreover, silane treatment alone seems to be very effective to improve bond strengths to ceramic. Thus, when the try-in step is involved, it should rather be done after silanation, followed by ultrasonic cleanse for better bond strength. A durable bond with high-strength polycrystalline ceramic systems has been proved to be a difficult task. The use of a silane-coupling agent after airborne particle abrasion
Cements and Adhesives 325(APA) did not result in a durable resin bond to zirconium.75,76 As an alternative, silicoat-ing has been proposed to create an additional silica layer over the reinforced ceramiccores to allow for bonding procedures. However, some reports demonstrated a signif-icant reduction in the bond strength after simulated artificial aging in zirconium-basedceramics treated with silicoating followed by silanization.75,77,78 Reinforced ceramiccore systems are not as dependent on bonding as the fragile feldspathic ceramics.Manufacturers’ recommendations for luting reinforced ceramic cores suggest theuse of conventional cements such as zinc phosphate or resin-modified glass ionomer.However, adhesive cementation has been shown to increase its fracture resistanceand longevity79,80; sealing of internal surface flaws created by airborne particle abra-sion (APA)81; and working as auxiliary retention to its inherent loose fit. Many different chemo-mechanical surface treatments have demonstrated effective-ness in optimizing the cement/reinforced ceramic bonding interface.82–84 Slight differ-ences in the sintering temperature may influence the final poly-crystal structure, grainsizes, and mechanical properties. Thus, different ceramics reactions to specificsurface treatments may be expected.82 Several studies have investigated if thesetreatments, combined or not, can promote more durable bonds to reinforced ceramiccores. Among them, there is airborne particle abrasion (APA) or wet hand grinding, useof phosphate ester and phosphoric acid monomers present either in resin lutingcements or some primers; tribochemical silicoating, laser irradiation, selective infiltra-tion–etching (SIE) technique by heat treatment, and others. To date, however, there isno clinical consensus regarding the best surface conditioning method for achievingoptimum bond strength to reinforced ceramics. Despite these invaluable efforts, theclinical significance of bonding to high-strength ceramics and its influence on thelong-term survival warrants future investigation.APA APA or wet hand grinding is an alternative widely investigated for improved resinbonding to reinforced ceramics.83 Some research groups have demonstrated thatthese mechanical surface modifications significantly increased the flexural strengthof Yttria-stabilized tetragonal zirconia polycrystal (Y-TZP)83,85–87 by inducing a tetrag-onal to monolithic phase transformation that could inhibit microcrack extension, thusincreasing the strength of zirconium. Conversely, other scientific evidences areshowing that surface treatments such as grinding or sandblasting Y-TZP ceramicsbefore cementation may create surface defects and sharp cracks that can be stressconcentration sources that render the zirconium framework susceptible to radialcracking during function.88,89 Significantly lower reliability for zirconium core ceramicswas demonstrated for two postsintered cementation surface modification techniques,grinding andalumina abrasion, when compared with the as-received zirconiumcores.90 In 2005, Guazzato and colleagues85 detected a significant amount of mono-clinic phase (9.5%) after sandblasting but no monoclinic phase detection after heattreatment. Authors assumed that the compressive stresses created were released,and the mean flexural strength obtained was related to the defects induced by sand-blasting without the benefits of the transformed region. Thus, they assumed that anytemporary beneficial effect induced by different surface treatment methods could becounteracted by fatigue-related crack growth phenomena.85 Low-pressure air abrasion (0.05 MPa) was proposed as an alternative to improvebond strength91,92 without compromising the ceramic structure. The authors of bothstudies stated that although the surface roughness was reduced, it did not affectthe long-term bond strength. However, omitting air abrasion resulted in debondingduring artificial aging, independent of using primers.91 In 2010, Aboushelib andcolleagues93 demonstrated that APA specimens may have their flexural strength
326 Manso et al recovered by the application of the bonding agent. Standard error of the mean anal- ysis of the fractured surfaces indicated that application of the bonding agent resulted in sealing of the surface damage produced by APA. Additionally, Casucci and colleagues82 (2010) evaluated the surface roughness for three different ceramics and a significant increase in the average surface roughness of Cercon (DETREY DENTSPLY) (DeguDent, Hanau, Germany) and Aadva (GC Corporation, Tokyo, Japan) Zr ceramics were found, while no differences were produced on Lava (3M ESPE, St Paul, MN, USA). Thus, manufacturers’ recommendations must be taken under consid- eration regarding APA and wet grinding mechanical surface modification, because ceramics perform differently in response to the same APA approach. Resin cements and primers containing 10-MDP monomer (10-methacryloyloxy- decyl dihydrogenphosphate) have been considered the materials of choice because of the chemical interaction established between the hydroxyl groups of the zirconia ceramic and the phosphate ester monomer of the MDP-containing material.94,95 Resin luting cements as Panavia,96 and some primers as Alloy Primer, Clearfil Ceramic Primer (Kuraray, Osaka, Japan) are representatives of this type of material. The use of zirconia 10-MDP-based primers in combination with APA improved resin bond strength, immediately and in long-term evaluations.78,83,91,97,98 However, more recently, Aboushelib and colleagues93 observed bond strength reduction after artificial aging for the APA group in combination with application of MDP monomer. Authors93 related the contradiction to the fact that their study used microbars instead of discs, which expose more surface area of the bonded interface to the influence of water. Primers containing phosphoric acid monomer as Metal/Zirconia Primer (Ivoclar-Viva- dent) and AZ Primer (Shofu) are also considered alternative to promote the adhesion to oxide ceramics such as zirconia and alumina, because they are claimed to achieve chemical bond to the oxidic ceramic surface.91,97 Differences in chemical composition of the primers and their bonding mechanisms require adequate combination of surface treatments and the proper selection of primer according to each commercial resin cement system.98 In general, primers containing a phosphonic acid monomer or phosphate ester monomer improve resin bonding to zirconia ceramics, while primers containing a silane-coupling agent improve resin bonding to silica–base ceramics.97 A new zirconia experimental primer, based on a mixture of organophosphate and carboxylic acid monomers, has been recently investigated as another alternative to increase bond strength of different resin-based luting agents.99 Tribochemical silicoating Tribochemical silicoating has been claimed as an alternative to APA, in an attempt to improve the bond between alumina/zirconia ceramics and resin cements.100 In this technique, the surfaces are airborne-particle abraded with aluminum trioxide particles modified with silica. The blasting pressure results in the embedding of the silica-coated alumina particles on the ceramic surface, rendering the silica-modified surface chemically reactive to the resin through silane-coupling agents. Some studies have demonstrated high bond strength values of resin to zirconia after silicoating and silanation.83,101 However, when artificial aging was proposed, it resulted in significant decrease in bond strengths of resin to silicoated zirconia.76–78 The authors further indicated that thermal cycling had a greater impact on the durability of the resin bond to zirconia ceramic than water storage at constant temperature.76–78 New approaches to enhance bonds to high-strength polycrystalline ceramics A newly developed surface treatment has been proposed to improve zirconia bonding, the selective infiltration etching (SIE) technique by heat treatment.93 It transforms the zirconia from a dense, nonretentive, and low-energy surface to a highly active and retentive surface. In this procedure, the surface is coated with a glass-containing
Cements and Adhesives 327conditioning agent (composed of silica, alumina, sodium oxide potassium oxide, andtitanium oxide) and heated above its glass transition temperature. After cooling, theglass is dissolved in an acidic bath, creating a porous surface and achieving promisingresults in terms of bond strength to resin cements. In 2010, Aboushelib andcolleagues93 demonstrated that SIE established a strong, stable, and durable bondto zirconia substrates as well. Stanard error of the mean analysis demonstrated thatthe surface topography created a highly retentive surface where the adhesive resinpenetrated and interlocked. Even though the depth of resin tags was limited to 0.3 mmto 0.7mm, the porosities allowed for the establishment of a strong nanomechanicalbond with the adhesive resin used, which resisted nanoleakage during artificial aging.93 Alternatively, laser irradiation has been introduced as another treatment option forzirconia and alumina surfaces. Er,Cr:YSGG laser should be considered an innovativealternative for promoting adhesion of ceramics (glass-infiltrated alumina) to resincement, since it resulted in similar bond strength values compared with the tribochem-ical treatment.102 Also, CO2 laser etching may represent an effective method forconditioning zirconia surfaces, enhancing micromechanical retention, and improvingthe bond strength of resin cement on zirconia ceramic.84SUMMARYClinical trials are required to understand what the real performance of new ceramics inthe oral environment may be and what the role of luting agents and surface treatmentson their performance may be. In addition, many other individual factors are involved ina clinical failure, such as core design and thickness and damage by processing andhandling, added to the occlusal function. The high number of clinical complicationswith all-ceramic fixed dental prostheses, even with increased connector size,103requires clinical attention in the material selection, and an important improvement ofthe veneering system is still required.104 Up to date, there are a limited number of pub-lished clinical trials on Y-TZP and other reinforced core ceramics, but it has the poten-tial for being accepted as a suitable material for fixed prosthodontics.105 In addition, it is important to evaluate the long-term performance of different surfacetreatments. Other approaches are expected to be developed to improve/stabilize thebonding mechanisms to teeth and all-ceramic systems involving, for instance, chem-ical function of the tooth and ceramic substrates via increase of the amount of –OHgroups and consequently the wet ability response on the surfaces prior bonding,potentially enhancing the long-term expectation of ceramic/cement/substrateinterface.ACKNOWLEDGMENTS The authors thank Dr Van Thompson, chair of the department of Biomaterials andBiomimetics at New York University College of Dentistry for his guidance and editorialsupport.REFERENCES 1. Meyer JM, Cattani-Lorente MA, Dupuis V. Compomers: between glass–ionomer cements and composites. Biomaterials 1998;19(6):529–39. 2. Rosenstiel SF, Land MF, Crispin BJ. Dental luting agents: a review of the current literature. J Prosthet Dent 1998;80(3):280–301. 3. O’Brien W. Dental materials and their selection. 3rd edition. Chicago (IL): Quin- tessence; 2002. p. 133–55.
328 Manso et al 4. Wettstein F, Sailer I, Roos M, et al. Clinical study of the internal gaps of zirconia and metal frameworks for fixed partial dentures. Eur J Oral Sci 2008;116(3):272–9. 5. Yiu CK, Tay FR, King NM, et al. Interaction of glass–ionomer cements with moist dentin. J Dent Res 2004;83(4):283–9. 6. Glasspoole EA, Erickson RL, Davidson CL. Effect of surface treatments on the bond strength of glass ionomers to enamel. Dent Mater 2002;8:454–62. 7. Naasan MA, Watson TF. Conventional glass ionomers as posterior restorations. A status report for the American Journal of Dentistry. Am J Dent 1998;11(1): 36–45. 8. Kerby RE, Knobloch L. Strength characteristics of glass–ionomer cements. Oper Dent 1992;17(5):170–4. 9. Peumans M, Van Meerbeek B, Lambrechts P, et al. Porcelain veneers: a review of the literature. J Dent 2000;28(3):163–77. 10. Christensen GJ. The rise of resin for cementing restorations. J Am Dent Assoc 1993;124(10):104–5. 11. Breeding LC, Dixon DL, Caughman WF. The curing potential of light-activated composite resin luting agents. J Prosthet Dent 1991;65(4):512–8. 12. Caughman WF, Chan DC, Rueggeberg FA. Curing potential of dual- polymerizable resin cements in simulated clinical situations. J Prosthet Dent 2001;86(1):101–6. 13. Myers ML, Caughman WF, Rueggeberg FA. Effect of restoration composition, shade, and thickness on the cure of a photoactivated resin cement. J Prostho- dont 1994;3(3):149–57. 14. Anusavice KJ. Phillips’ science of dental materials. 11th edition. Philadelphia: Saunders Elsevier; 2003. 15. Mitra SB. Dental cements: formulations and handling techniques. In: Curtis VR, Watson T, editors. Dental biomaterials. Imaging, testing, and modeling. Boca Raton (FL): Woodhead Publishing Limited and CRC Press LLC; 2008. p. 27. 16. el-Badrawy WA, el-Mowafy OM. Chemical versus dual curing of resin inlay cements. J Prosthet Dent 1995;73(6):515–24. 17. Hasegawa EA, Boyer DB, Chan DC. Hardening of dual-cured cements under composite resin inlays. J Prosthet Dent 1991;66(2):187–92. 18. Pereira SG, Fulgencio R, Nunes TG, et al. Effect of curing protocol on the poly- merization of dual-cured resin cements. Dent Mater 2010;26(7):710–8. ¸˜ ¸˜ 19. Pegoraro TA. Efeito do protocolo de ativacao da polimerizacao e envelhecimen- to acelerado em algumas propriedades de cimentos resinosos. Bauru (Brazil): ¸˜ Reabilitacao Oral, Faculdade de Odontologia de Bauru, Universidade de Sao ˜ Paulo; 2010 [in Portuguese]. 20. Pegoraro TA, da Silva NR, Carvalho RM. Cements for use in esthetic dentistry. Dent Clin North Am 2007;51(2):453–71. 21. Peutzfeldt A, Asmussen E. Investigations on polymer structure of dental resinous materials. Trans Acad Dent Mater 2004;18:81–104. 22. Carvalho RM, Garcia FC, e Silva SM, et al. Adhesive–composite incompatibility, part II. J Esthet Restor Dent 2005;17(3):191–5. 23. Tay FR, Pashley DH, Yiu CK, et al. Factors contributing to the incompatibility between simplified-step adhesives and chemically cured or dual-cured composites. Part I. Single-step self-etching adhesive. J Adhes Dent 2003; 5(1):27–40. 24. Tay FR, Suh BI, Pashley DH, et al. Factors contributing to the incompatibility between simplified-step adhesives and self-cured or dual-cured composites. Part II. Single-bottle, total-etch adhesive. J Adhes Dent 2003;5(2):91–105.
Cements and Adhesives 32925. Cheong C, King NM, Pashley DH, et al. Incompatibility of self-etch adhesives with chemical/dual-cured composites: two-step vs one-step systems. Oper Dent 2003;28(6):747–55.26. Sanares AM, Itthagarun A, King NM, et al. Adverse surface interactions between one-bottle light-cured adhesives and chemical-cured composites. Dent Mater 2001;17(6):542–56.27. Suh BI, Feng L, Pashley DH, et al. Factors contributing to the incompatibility between simplified-step adhesives and chemically cured or dual-cured compos- ites. Part III. Effect of acidic resin monomers. J Adhes Dent 2003;5(4):267–82.28. Carvalho RM, Pegoraro TA, Tay FR, et al. Adhesive permeability affects coupling of resin cements that utilise self-etching primers to dentine. J Dent 2004;32(1): 55–65.29. Tay FR, Pashley DH, Suh BI, et al. Single-step adhesives are permeable membranes. J Dent 2002;30:371–82.30. King NM, Tay FR, Pashley DH, et al. Conversion of one-step to two-step self-etch adhesives for improved efficacy and extended application. Am J Dent 2005; 18(2):126–34.31. Cury AH, Goracci C, de Lima Navarro MF, et al. Effect of hygroscopic expansion on the push-out resistance of glass ionomer-based cements used for the luting of glass fiber posts. J Endod 2006;32(6):537–40.32. Goracci C, Fabianelli A, Sadek FT, et al. The contribution of friction to the dislo- cation resistance of bonded fiber posts. J Endod 2005;31(8):608–12.33. Paul SJ, Scharer P. The dual bonding technique: a modified method to improve adhesive luting procedures. Int J Periodontics Restorative Dent 1997;17(6): 536–45.34. Duarte S Jr, de Freitas CR, Saad JR, et al. The effect of immediate dentin sealing on the marginal adaptation and bond strengths of total-etch and self-etch adhe- sives. J Prosthet Dent 2009;102(1):1–9.35. Hu J, Zhu Q. Effect of immediate dentin sealing on preventive treatment for post- cementation hypersensitivity. Int J Prosthodont 2010;23(1):49–52.36. Duke ES. New technology directions in resin cements. Compend Contin Educ Dent 2003;24(8). 606–8, 610.37. Burke FJ, Crisp RJ, Richter B. A practice-based evaluation of the handling of a new self-adhesive universal resin luting material. Int Dent J 2006;56(3): 142–6.38. Radovic I, Monticelli F, Goracci C, et al. Self-adhesive resin cements: a literature review. J Adhes Dent 2008;10(4):251–8.39. De Munck J, Van Landuyt K, Peumans M, et al. A critical review of the durability of adhesion to tooth tissue: methods and results. J Dent Res 2005;84(2):118–32.40. Gerth HU, Dammaschke T, Zuchner H, et al. Chemical analysis and bonding reaction of RelyX Unicem and Bifix composites—a comparative study. Dent Mater 2006;22(10):934–41.41. Abo-Hamar SE, Hiller KA, Jung H, et al. Bond strength of a new universal self- adhesive resin luting cement to dentin and enamel. Clin Oral Investig 2005;9(3): 161–7.42. Hikita K, Van Meerbeek B, De Munck J, et al. Bonding effectiveness of adhesive luting agents to enamel and dentin. Dent Mater 2007;23(1):71–80.43. De Munck J, Vargas M, Van Landuyt K, et al. Bonding of an autoadhesive luting material to enamel and dentin. Dent Mater 2004;20(10):963–71.44. Al-Assaf K, Chakmakchi M, Palaghias G, et al. Interfacial characteristics of adhe- sive luting resins and composites with dentine. Dent Mater 2007;23(7):829–39.
330 Manso et al 45. Flury S, Lussi A, Peutzfeldt A, et al. Push-out bond strength of CAD/CAM- ceramic luted to dentin with self-adhesive resin cements. Dent Mater 2010; 26(9):855–63. 46. Guarda GB, Goncalves LS, Correr AB, et al. Luting glass ceramic restorations using a self-adhesive resin cement under different dentin conditions. J Appl Oral Sci 2010;18(3):244–8. 47. Tanoue N, Koishi Y, Atsuta M, et al. Properties of dual-curable luting composites polymerized with single and dual curing modes. J Oral Rehabil 2003;30(10): 1015–21. 48. Fan PL, Edahl A, Leung RL, et al. Alternative interpretations of water sorption values of composite resins. J Dent Res 1985;64(1):78–80. 49. Ortengren U, Elgh U, Spasenoska V, et al. Water sorption and flexural properties of a composite resin cement. Int J Prosthodont 2000;13(2):141–7. 50. Oysaed H, Ruyter IE. Composites for use in posterior teeth: mechanical proper- ties tested under dry and wet conditions. J Biomed Mater Res 1986;20(2): 261–71. 51. Ferracane JL, Berge HX, Condon JR. In vitro aging of dental composites in water—effect of degree of conversion, filler volume, and filler/matrix coupling. J Biomed Mater Res 1998;42(3):465–72. 52. Huang M, Niu X, Shrotriya P, et al. Contact damage of dental multilayers: viscous deformation and fatigue mechanisms. J Eng Mater Technol 2005;127(33):33–9. 53. Braden M, Clarke RL. Water absorption characteristics of dental microfine composite filling materials. I. Proprietary materials. Biomaterials 1984;5(6): 369–72. 54. Pearson GJ, Longman CM. Water sorption and solubility of resin-based mate- rials following inadequate polymerization by a visible-light curing system. J Oral Rehabil 1989;16(1):57–61. 55. Vrochari AD, Eliades G, Hellwig E, et al. Water sorption and solubility of four self- etching, self-adhesive resin luting agents. J Adhes Dent 2010;12(1):39–43. 56. Scherrer SS, de Rijk WG, Belser UC, et al. Effect of cement film thickness on the fracture resistance of a machinable glass–ceramic. Dent Mater 1994;10(3): 172–7. 57. Magne P, Kwon KR, Belser UC, et al. Crack propensity of porcelain laminate veneers: a simulated operatory evaluation. J Prosthet Dent 1999;81(3):327–34. 58. Silva NR, de Souza GM, Coelho PG, et al. Effect of water storage time and composite cement thickness on fatigue of a glass–ceramic trilayer system. J Biomed Mater Res B Appl Biomater 2008;84(1):117–23. 59. Cekic-Nagas I, Canay S, Sahin E. Bonding of resin core materials to lithium dis- ilicate ceramics: the effect of resin cement film thickness. Int J Prosthodont 2010;23(5):469–71. 60. Van Noort R. Introduction to dental materials. 3rd edition. London: Mosby Elsevier; 2007. 61. Raigrodski AJ, Chiche GJ. All-ceramic fixed partial dentures. Part I: in vitro studies. J Esthet Restor Dent 2002;14(3):188–91. 62. Raigrodski AJ, Chiche GJ, Potiket N, et al. The efficacy of posterior three-unit zirconium-oxide-based ceramic fixed partial dental prostheses: a prospective clinical pilot study. J Prosthet Dent 2006;96(4):237–44. 63. Raigrodski AJ, Chiche GJ, Swift EJ Jr. All-ceramic fixed partial dentures. Part III: clinical studies. J Esthet Restor Dent 2002;14(5):313–9. 64. Sailer I, Feher A, Filser F, et al. Five-year clinical results of zirconia frameworks for posterior fixed partial dentures. Int J Prosthodont 2007;20(4):383–8.
Cements and Adhesives 33165. Sailer I, Philipp A, Zembic A, et al. A systematic review of the performance of ceramic and metal implant abutments supporting fixed implant reconstructions. Clin Oral Implants Res 2009;20(Suppl 4):4–31.66. Sailer I, Pjetursson BE, Zwahlen M, et al. A systematic review of the survival and complication rates of all-ceramic and metal–ceramic reconstructions after an observation period of at least 3 years. Part II: fixed dental prostheses. Clin Oral Implants Res 2007;18(Suppl 3):86–96.67. Tinschert J, Schulze KA, Natt G, et al. Clinical behavior of zirconia-based fixed partial dentures made of DC-Zirkon: 3-year results. Int J Prosthodont 2008; 21(3):217–22.68. Clelland NL, Warchol N, Kerby RE, et al. Influence of interface surface condi- tions on indentation failure of simulated bonded ceramic onlays. Dent Mater 2006;22(2):99–106.69. Blatz MB, Sadan A, Kern M. Resin–ceramic bonding: a review of the literature. J Prosthet Dent 2003;89(3):268–74.70. Barghi N, Chung K, Farshchian F, et al. Effects of the solvents on bond strength of resin-bonded porcelain. J Oral Rehabil 1999;26(11):853–7.71. Hooshmand T, van Noort R, Keshvad A. Bond durability of the resin-bonded and silane-treated ceramic surface. Dent Mater 2002;18(2):179–88.72. Meng XF, Yoshida K, Gu N. Chemical adhesion rather than mechanical retention enhances resin bond durability of a dental glass–ceramic with leucite crystal- lites. Biomed Mater 2010;5(4):044101.73. Ishida H. Structural gradient in the silane-coupling agent layers and its influence on the mechanical and physical properties of composites. New York (NY): Plenum Press; 1985. p. 25–50.74. Hooshmand T, van Noort R, Keshvad A. Storage effect of a preactivated silane on the resin to ceramic bond. Dent Mater 2004;20(7):635–42.75. Derand T, Molin M, Kvam K. Bond strength of composite luting cement to zirconia ceramic surfaces. Dent Mater 2005;21(12):1158–62.76. Kern M, Wegner SM. Bonding to zirconia ceramic: adhesion methods and their durability. Dent Mater 1998;14(1):64–71.77. Ozcan M, Vallittu PK. Effect of surface conditioning methods on the bond strength of luting cement to ceramics. Dent Mater 2003;19(8):725–31.78. Wegner SM, Kern M. Long-term resin bond strength to zirconia ceramic. J Adhes Dent 2000;2(2):139–47.79. Della Bona A, Kelly JR. The clinical success of all-ceramic restorations. J Am Dent Assoc 2008;139:8S–13S.80. Scherrer SS, De Rijk WG, Belser UC. Fracture resistance of human enamel and three all-ceramic crown systems on extracted teeth. Int J Prosthodont 1996;9(6): 580–5.81. Blatz MB. Long-term clinical success of all-ceramic posterior restorations. Quin- tessence Int 2002;33(6):415–26.82. Casucci A, Mazzitelli C, Monticelli F, et al. Morphological analysis of three zirco- nium oxide ceramics: effect of surface treatments. Dent Mater 2010;26(8): 751–60.83. Qeblawi DM, Munoz CA, Brewer JD, et al. The effect of zirconia surface treat- ment on flexural strength and shear bond strength to a resin cement. J Prosthet Dent 2010;103(4):210–20. ¨ ¨ ¨ ¨84. Ural XC, Kulunk T, Kulunk S, et al. Determination of resin bond strength to zirconia ceramic surface using different primers. Acta Odontol Scand 2010; 69:48–53.
332 Manso et al 85. Guazzato M, Quach L, Albakry M, et al. Influence of surface and heat treatments on the flexural strength of Y-TZP dental ceramic. J Dent 2005;33(1):9–18. 86. Kosmac T, Oblak C, Jevnikar P, et al. The effect of surface grinding and sand- blasting on flexural strength and reliability of Y-TZP zirconia ceramic. Dent Mater 1999;15(6):426–33. 87. Kosmac T, Oblak C, Jevnikar P, et al. Strength and reliability of surface treated Y-TZP dental ceramics. J Biomed Mater Res 2000;53(4):304–13. 88. Lawn BR, Deng Y, Lloyd IK, et al. Materials design of ceramic-based layer struc- tures for crowns. J Dent Res 2002;81(6):433–8. 89. Zhang Y, Lawn BR, Rekow ED, et al. Effect of sandblasting on the long-term performance of dental ceramics. J Biomed Mater Res B Appl Biomater 2004; 71(2):381–6. 90. Guess PC, Zhang Y, Kim JW, et al. Damage and reliability of Y-TZP after cemen- tation surface treatment. J Dent Res 2010;89(6):592–6. 91. Kern M, Barloi A, Yang B. Surface conditioning influences zirconia ceramic bonding. J Dent Res 2009;88(9):817–22. 92. Yang B, Barloi A, Kern M. Influence of air-abrasion on zirconia ceramic bonding using an adhesive composite resin. Dent Mater 2010;26(1):44–50. 93. Aboushelib MN, Feilzer AJ, Kleverlaan CJ. Bonding to zirconia using a new surface treatment. J Prosthodont 2010;19(5):340–6. 94. Oyague RC, Monticelli F, Toledano M, et al. Effect of water aging on microtensile bond strength of dual-cured resin cements to pretreated sintered zirconium- oxide ceramics. Dent Mater 2009;25(3):392–9. 95. Tanaka R, Fujishima A, Shibata Y, et al. Cooperation of phosphate monomer and silica modification on zirconia. J Dent Res 2008;87(7):666–70. 96. Blatz MB, Sadan A, Martin J, et al. In vitro evaluation of shear bond strengths of resin to densely sintered high-purity zirconium oxide ceramic after long-term storage and thermal cycling. J Prosthet Dent 2004;91(4):356–62. 97. Kitayama S, Nikaido T, Takahashi R, et al. Effect of primer treatment on bonding of resin cements to zirconia ceramic. Dent Mater 2010;26(5):426–32. 98. Yun JY, Ha SR, Lee JB, et al. Effect of sandblasting and various metal primers on the shear bond strength of resin cement to Y-TZP ceramic. Dent Mater 2010; 26(7):650–8. 99. Magne P, Paranhos MP, Burnett LH Jr. New zirconia primer improves bond strength of resin-based cements. Dent Mater 2010;26(4):345–52. 100. Kern M, Thompson VP. Sandblasting and silica coating of a glass-infiltrated alumina ceramic: volume loss, morphology, and changes in the surface compo- sition. J Prosthet Dent 1994;71(5):453–61. 101. Kim BK, Bae HE, Shim JS, et al. The influence of ceramic surface treatments on the tensile bond strength of composite resin to all-ceramic coping materials. J Prosthet Dent 2005;94(4):357–62. 102. de Paula Eduardo C, Bello-Silva MS, Moretto SG, et al. Microtensile bond strength of composite resin to glass-infiltrated alumina composite conditioned with Er, Cr:YSGG laser. Lasers Med Sci 2010. [Epub ahead of print]. 103. Land MF, Hopp CD. Survival rates of all-ceramic systems differ by clinical indi- cation and fabrication method. J Evid Based Dent Pract 2010;10(1):37–8. 104. Schley JS, Heussen N, Reich S, et al. Survival probability of zirconia-based fixed dental prostheses up to 5 yr: a systematic review of the literature. Eur J Oral Sci 2010;118(5):443–50. 105. Al-Amleh B, Lyons K, Swain M. Clinical trials in zirconia: a systematic review. J Oral Rehabil 2010;37(8):641–52.